REVIEW OF PITTING CORROSION FATIGUE MODELS
Prof. D.W. Hoeppner1
Dr. V. Chandrasekaran2
Ms. A.M.H. Taylor3
The combined effect of corrosion and cyclic loading have been
shown to produce cracks from corrosion pits and pits have
frequently been the source of cracks on aircraft components
operating in fleets. Once the pit or group of pits form, the rate of
pit growth is dependent mainly on the material, environmental
conditions, and type and state of stress. Therefore, to estimate the
total corrosion fatigue life of a component, it is of great importance
to develop realistic models to establish the component life in these
situations and to formulate methods by which designers and
operators know likely sources of pitting early in the design and
fleet operation. Therefore, to understand this phenomena, some
models based on pitting corrosion fatigue (PCF) mechanisms
and understanding have been proposed in the past and new ones
It is important to note that both pitting theory and crack growth
theory have been used in pitting corrosion fatigue model
development. The first known conceptual (notional) model was
presented in 1971 and subsequently the pit growth rate theory
proposed by Godard was combined with fatigue crack growth
concepts. Following this basic idea, a few models have been
This paper presents some examples of critical pitting corrosion
fatigue situations in aircraft, discusses the framework of the PCF
models to date, presents some applications of the models, and
discusses current work underway. Additionally, some
recommendations are made related to future work needed to
enhance structural integrity and degradation of aircraft from this
The phases of life of a structure may be classified as follows (1):
1 Professor and Director, Quality and Integrity Design Engineering Center (QIDEC), Mechanical
Engineering Department, University of Utah, Salt Lake City, Utah 84112.
2 Research Assistant Professor, Mechanical Engineering Department, University of Utah, Salt Lake City,
3 Research Engineer, Mechanical Engineering Department, University of Utah, Salt Lake City, Utah 84112.
• Nucleation or formation of damage by a specific, physical or corrosion damage
process interacting with the fatigue process if appropriate. Corrosion and other
processes may act alone to create the damage. a transition from the nucleation stage
to the next phase must occur. Phase L1.
• Microstructurally dominated crack linkup and propagation (“short” or “small” crack
regime). Phase L2.
• Crack propagation in the regime where either LEFM, EPFM, or FPFM may be
applied both for analysis and material characterization (the “long” crack regime).
• Final instability. Phase L4.
Thus, the total life (LT) of a structure is LT = L1+L2+L3+L4. Figure 1 presents a
depiction of the degradation process. The regions shown, e.g. 1, 2, 3, and 4, illustrate the
portion of life, on the abscissa, and the corresponding growth in discontinuity size plotted
schematically on the ordinate. This paper concentrates on the phases L1 and L2. That is,
the corrosion process that results in the generation of a specific form of corrosion
generating a specific form of discontinuity that is not necessarily a crack like
discontinuity, and the development of short cracks and their propagation. The
requirement of the community to come up with design methods to deal with corrosion or
other degradation, fatigue, creep, and wear, is essential and some of the elements are
depicted in Figure 2. This figure illustrates that most of the quantitative methods that
have been developed used the concepts of mechanics of materials with an incorporation
of fracture mechanics (2).
EFFECTS OF CORROSION ON STRUCTURAL INTEGRITY OF AIRCRAFT
The issue of the effects of corrosion on structural integrity of aircraft has been a
question of concern for some time (3-38). The potential effects are many and they can be
categorized as follows. In the discussion below the use of the terms global and local
refers to the likely extent of the corrosion on the surface of a component. Global means
the corrosion would be found on much of the component whereas local means the
corrosion may be localized to only small, local areas.
1) Reduce the section with a concomitant increase in stress. Global or local.
2) Produce a stress concentration. Local.
3) Nucleate cracks. Local, possibly global. Source of Multiple-site cracking.
4) Produce corrosion debris. This may result in surface pillowing by various means,
which may significantly change the stress state and structural behavior. Local and
5) Create a situation that causes the surfaces to malfunction. Local and global.
6) Cause environmentally assisted crack growth (EACG) under cyclic (Corrosion
fatigue) or sustained loading (SCC) conditions. Local.
7) Create a damage state that is missed in inspection when the inspection plan was
not developed for corrosion or when corrosion is missed. Local and global.
8) Change the structurally significant item due to the creation of a damage state not
envisioned in the structural damage analysis or fatigue and strength analysis. If
the SSI is specified, for example, by location of maximum stress or strain, then
the corrosion may cause another area(s) to become significant. Local or global.
9) Create an embrittlement condition in the material that subsequently affects
behavior. Local or Global.
10) Create a general aesthetic change from corrosion that creates maintenance to be
done and does damage to the structure. Local or global.
11) Corrosion maintenance does not eliminate all the corrosion damage and cracking
or the repair is specified improperly or executed improperly thus creating a
damage state not accounted for in the design. Local or global.
12) Generate a damage state that alters either the durability phase of life or the
damage tolerant assessment of the structure or both.
13) Create a widespread corrosion damage (WCD) state or a state of corrosion that
impacts the occurrence of widespread fatigue damage (WFD) and its concomitant
effects. (See references 3, 5, 6, 15, 17, 28, 29, 30, 34, 35, 36, 37, 38 for more
The question of whether corrosion, corrosion fatigue and stress corrosion cracking are
safety concerns or just maintenance/economic concerns has been a point of discussion
related to aircraft structural integrity for over 30 years. Nonetheless, a great deal of the
aircraft structural integrity community believes that corrosion related degradation is just
an economic concern. It was with this situation in mind that Campbell and Lehay (14)
and Wallace, Hoeppner and Kandachar (15) pursued the presentation of technical facts
and knowledge to illustrate the potential for a safety issue as well as a
maintenance/economic issue. Finally, Hoeppner et al (30) at the 1995 ICAF meeting in
Melbourne, Australia reviewed failure data obtained from the USAF, USN, US Army,
FAA, and the NTSB related to aircraft incidents and accidents in the USA between 1975-
1994 to evaluate further the potential for corrosion and fretting related degradation to be
significant safety issues. Recently, several instances of pitting corrosion in aircraft and
helicopter components have been identified as critical safety issues as discussed in the
EXAMPLES OF PITTING CORROSION INCIDENTS
A survey was performed of incidents and accidents of aircraft and helicopters
caused by pitting corrosion, where an incident is any damage to the aircraft and/or
injuries to passengers and crew and an accident is loss of the aircraft and/or fatal injuries
to passengers and crew. Data were taken from the NTSB and FAA web-sites, which
include their databases of all aircraft incidents and accidents since 1983. It was
determined that of the 91 incidents and accidents found under corrosion, seven of those
gave the cause of failure as pitting corrosion.
Unfortunately, it has been found that there are problems in reporting the causes of
the incidents and accidents in the NTSB and FAA in that the real cause of an incident or
accident is not reported properly and, therefore, does not show up in the database. For
example, in reading through some of the incidents and accidents caused by corrosion, it
was found in the text that the real cause of failure was, more specifically, due to pitting
corrosion or exfoliation. But those words were not highlighted so that incident or
accident did not show up in a search of pitting corrosion or exfoliation. This makes the
validity of numbers of incidents and accidents caused by pitting corrosion questionable
due to the fact that additional incidents and accidents may be listed under different causes
and/or more general causes. Also included in the survey were the three Embraer 120
incidents involving propeller blades, the Aero Commander 680 lower spar cap, and the F-
18 trailing edge flap failure. These civilian and military incidents and accidents were all
due to pitting corrosion as shown in Table 1. When these examples are taken with the
general information cited in the previous references they clearly show that corrosion
related degradation is a significant safety issue in the assurance of structural integrity of
Therefore, the potential regrettable occurrence of accidents from corrosion related
crack nucleation is a constant threat to aircraft safety. The following quote from the
recent NATO RTO conference on fatigue in the presence of corrosion adds some